Mechanical properties and drug release behavior of PCL/zein coated 45S5 bioactive glass scaffolds for bone tissue engineering application

This article presents data related to the research article entitled “The effect of coating type on mechanical properties and controlled drug release of PCL/zein coated 45S5 bioactive glass scaffolds for bone tissue engineering” [1]. We provide data on mechanical properties, in vitro bioactivity and drug release of bioactive glass (BG) scaffolds coated by poly (ε-caprolactone) (PCL) and zein used as a controlled release device for tetracycline hydrochloride (TCH). By coating the BG scaffolds with PCL or PCL/zein blend the mechanical properties of the scaffolds were substantially improved, i.e., the compressive strength increased from 0.004±0.001 MPa (uncoated BG scaffolds) to 0.15±0.02 MPa (PCL/zein coated BG scaffolds). A dense bone-like apatite layer formed on the surface of PCL/zein coated scaffolds immersed for 14 days in simulated body fluid (SBF). The data describe control of drug release and in vitro degradation behavior of coating by engineering the concentration of zein. Thus, the developed scaffolds exhibit attractive properties for application in bone tissue engineering research.


a b s t r a c t
This article presents data related to the research article entitled "The effect of coating type on mechanical properties and controlled drug release of PCL/zein coated 45S5 bioactive glass scaffolds for bone tissue engineering" [1]. We provide data on mechanical properties, in vitro bioactivity and drug release of bioactive glass (BG) scaffolds coated by poly (ε-caprolactone) (PCL) and zein used as a controlled release device for tetracycline hydrochloride (TCH). By coating the BG scaffolds with PCL or PCL/zein blend the mechanical properties of the scaffolds were substantially improved, i.e., the compressive strength increased from 0.00470.001 MPa (uncoated BG scaffolds) to 0.1570.02 MPa (PCL/zein coated BG scaffolds). A dense bone-like apatite layer formed on the surface of PCL/zein coated scaffolds immersed for 14 days in simulated body fluid (SBF). The data describe control of drug release and in vitro degradation behavior of coating by engineering the concentration of zein. Thus, the developed scaffolds exhibit attractive properties for application in bone tissue engineering research. Value of the data

Contents lists available at
The data described here, PCL/zein composite as an organized innovative design coating, may be helpful to researchers who are interested in applications in in-situ drug release in bone tissue engineering.
Composite PCL/zein coated BG scaffolds with a novel type of drug controlled-release are shown. Compressive strength and mechanical stability are shown to be significantly increased via the optimized method for dip coating the BG scaffolds by PCL and zein.

Data, experimental design, materials and methods
The data provided here are stress-strain curves for uncoated and coated scaffolds with different concentration of PCL and zein before and after immersion in SBF for 28 days (Fig. 1) and drug release curves of BG scaffolds of uncoated and coated with PCL, PCL/zein and zein TCH-loaded (Fig. 2).

Polymer coating procedure and drug loading
In order to obtain a dual PCL/zein coating, PCL/zein (Sigma-Aldrich, USA) (50:50% w/w) solution was prepared by dissolving PCL in chloroform and zein in ethanol (Merck, Germany). Then, scaffolds were coated by this solution for two times. For the drug loading together with the PCL/zein polymer, TCH (0.5% w/v) was dissolved in ethanol solution and the coating procedure was performed similarly as for the unloaded coatings [1].   stress displacement curve, which is related to the work of fracture (toughness of the material). By increasing the concentration of polymer, the compressive strength of coated scaffolds was increased. The SEM images of PCL, PCL/zein and zein-coated scaffolds showed a smooth surface of the struts and no large microcracks present on scaffolds coated by PCL. Based on this data, the scaffold coated using a solution of 2.5% PCL: 2.5% zein w/v (1:1) was chosen for further investigation. The porosity and the compressive strength of the present coated scaffolds were $ 94% and 0.15 MPa, respectively. Fig. 1d shows the mechanical behavior of the PCL/zein coated scaffolds before and after immersion in SBF for 28 days. The compressive strength of the scaffolds decreased markedly during 28 days of immersion in SBF (0.094 70.004 MPa). The presence of bone-like apatite on the uncoated and coated scaffolds was confirmed by XRD, SEM and FTIR analyses. It is suggested that the PCL/zein coating will positively affect the bioactive character of 45S5 BG scaffolds. Indeed a cell biology assessment of the present scaffolds, in comparison to similar polymer coated BG scaffolds reported recently [5][6][7] remains to be carried out. The weight loss data of scaffolds are also increased by increasing the amount of zein. The weight loss for the PCL/zein (50:50) and zein films were 16% and 39%, respectively. It suggests that a majority of the zein component degraded after 28 days of immersion.

Drug release analysis
The absorbed drug within the coated scaffolds was released in a sustained manner over 10 days (Fig. 2). Three trends were observed for the drug release profiles: rapid, very slow and controlled drug released. The coated BG scaffolds containing zein have reduced release level compared to the uncoated and the coated scaffolds without protein. This data suggest that the entrapment of the drug by zein protein played an important role in the release behavior. The formation of protein-drug interactions is likely to contribute to the kinetics of the process, which should be related to the establishment of hydrogen bonds, van der Waals forces, and the release of solvent molecules [8,9]. The prediction of the actual mechanism is challenging. Some of the reasons that make such prediction difficult are related to the fact that the interactions also depend on the degradation rate of both components. In addition, there are difficulties for the evaluation of the enthalpy and entropic contribution of the solvent [9]. ATR-FTIR spectra of the TCH-loaded scaffolds are shown in the Supplementary data. To shed some light on the release rate of TCH from PCL/zein coated scaffolds a logarithmic function is fit to the experimental data. The function that we fit is D¼17.9 ln(t) À4.4785; where D is the cumulative drug release percentage and "t" is the release time in hours. The analysis of the data demonstrated that the total amount of TCH in PCL/zein coated scaffolds can be released after less than 15 days, as observed in previous researches [5,7,10].